### Liu, Shu (2016) Application of shakedown theory in the

### structural design of bituminous pavements. PhD thesis,

### University of Nottingham.

**Access from the University of Nottingham repository: **

http://eprints.nottingham.ac.uk/35577/1/thesis-final.pdf

**Copyright and reuse: **

The Nottingham ePrints service makes this work by researchers of the University of Nottingham available open access under the following conditions.

This article is made available under the University of Nottingham End User licence and may be reused according to the conditions of the licence. For more details see:

http://eprints.nottingham.ac.uk/end_user_agreement.pdf

**Application of Shakedown Theory in the **

**Structural Design of Bituminous **

**Pavements **

*by *

**Shu Liu**

*BEng*

### ,

* MSc*

### Thesis submitted to the University of Nottingham for

### the degree of Doctor of Philosophy

i

**ABSTRACT **

Excessive rutting, one of the major distress modes of bituminous pavements, is mainly caused by the accumulation of load-induced permanent deformation. However, current pavement design approaches against the excessive rutting are mainly developed using the theory of elasticity. Recently, a new pavement design approach based on the shakedown concept has attracted lots of attention because it can consider plastic properties of pavement materials. However, most of the existing shakedown solutions were developed for pavement foundations composed of granular materials and soils. Very limited work has been reported on bituminous pavements. Besides, current studies usually assume homogeneous, isotropic pavement materials obeying an associated plastic flow rule (termed as standard materials in the present study), which may not be realistic for pavement materials.

In the present research, a step-by-step numerical approach was used to obtain numerical shakedown limits of pavement structures under repeated moving loads. Both two-dimensional and three-dimensional problems were considered. It was found that, under the assumption of standard materials, the obtained numerical shakedown limits and residual stress fields agreed well with the available theoretical data.

A static (i.e. lower bound) shakedown approach for pavements with anisotropic, heterogeneous materials was developed based on Melan’s lower bound theorem

ii and the critical residual stress method of Yu and Wang (2012). The influence of material plastic flow rules on pavement shakedown limits was also evaluated both numerically and theoretically. It was found that neglect of the inherent material properties (i.e. anisotropy, heterogeneity and non-associated plastic flow) could overestimate the real shakedown limits of bituminous pavements.

A series of tests were conducted to validate the shakedown concept for the responses of bituminous pavements under traffic loads. Two distinct phenomena corresponding to shakedown and non-shakedown were observed. Triaxial tests and uniaxial compression tests were also undertaken to obtain the stiffness and strength parameters, from which the theoretical shakedown limits can be calculated. Comparison between the experimental results and the theoretical solutions revealed that the current 3D shakedown approach for standard materials may overestimate capacities of bituminous pavements.

Finally, the lower bound shakedown approach was employed to design a typical bituminous pavement. A direct comparison was made between the shakedown-based design and the current UK design method. It demonstrated that the shakedown-based design for bituminous pavements can be conducted considering the maximum contact pressure and a relatively high air temperature.

iii

**ACKNOWLEDGEMENTS **

First, I would like to express my sincere gratitude to my supervisors, Dr Dariusz Wanatowski, Professor Hai-Sui Yu and Dr. Juan Wang for their patience, motivation and continuous support of my Ph.D study over these years.

In addition, I need to thank Dr. Mostapha Boulbibane for the opportunity provided by him.

I also would like to thank Dr. Nick Thom, Dr. James Grenfell and all the technicians in the Nottingham Transportation Engineering Centre (NTEC) and L2 at the University of Nottingham who gave valuable advice in experimental design and specimen preparation.

I am also appreciative to express my gratitude to all my colleagues and friends for their sincere help and continuous encouragement.

Furthermore, I would like to acknowledge the financial support provided by the faculty of Engineering and the Graduate school at the University of Nottingham UK and Malaysia.

Finally, huge appreciation goes to my family and my boyfriend for their generous dedication and endless love.

iv

**CONTENTS **

ABSTRACT ... i
ACKNOWLEDGEMENTS ... iii
CONTENTS ... iv
LIST OF FIGURES ... x
LIST OF TABLES ... xix

NOTATION ... xxii

CHAPTER 1 INTRODUCTION ... 1

1.1 Background ... 1

1.2 Aims and objectives ... 4

1.3 Thesis outline ... 4

CHAPTER 2 LITERATURE REVIEW ... 7

2.1 Introduction ... 7

2.2 Notion of shakedown in pavements ... 7

2.3 Shakedown theorems ... 8

v

2.3.2 Koiter’s kinematic shakedown theorem ... 9

2.4 Bituminous pavements ... 10

2.4.1 Typical structure of bituminous pavements ... 10

2.4.2 Failure modes of bituminous pavements ... 12

2.4.3 Current pavement design methods... 15

2.5 Properties of pavement materials ... 18

2.5.1 Granular materials ... 18

2.5.2 Asphalt ... 20

2.5.3 Associated and non-associated plastic flow rule ... 24

2.5.4 Material anisotropy ... 25

2.5.5 Material heterogeneity ... 26

2.6 Previous studies of shakedown in pavement engineering ... 27

2.6.1 Experimental observation of shakedown behaviour ... 27

2.6.2 Shakedown analyses in pavement engineering... 35

2.7 ABAQUS ... 40

CHAPTER 3 SHAKEDOWN ANALYSIS OF PAVEMENTS WITH STANDARD MATERIALS ... 43

3.1 Introduction ... 43

3.2 Two-dimensional pavement problems ... 44

vi

3.2.2 Numerical approach ... 45

3.2.3 Review of the lower boud shakedown approach for a half-space with standard materials (Yu and Wang 2012; Wang and Yu 2013b) ... 46

3.2.4 Model description ... 48

3.2.5 Model validation ... 49

3.2.6 Solutions and discussions ... 54

3.3 Three-dimensional pavement problems ... 70

3.3.1 Problem definition ... 70

3.3.2 Model description and verification ... 70

3.3.3 Solutions and discussions ... 72

3.4 Summary ... 77

CHAPTER 4 SHAKEDOWN ANALYSIS OF PAVEMENTS WITH MATERIALS FOLLOWING NON-ASSOCIATED PLASTIC FLOW ... 80

4.1 Introduction ... 80

4.2 Numerical shakedown analysis ... 81

4.2.1 General introduction ... 81

4.2.2 Solutions of single-layered pavements ... 82

4.2.3 Solutions of multi-layered pavements ... 89

4.3 Static shakedown analysis ... 95

vii 4.3.2 Static shakedown approach for pavements with materials

following non-associated plastic flow ... 95

4.3.3 Solutions of single-layered pavements ... 97

4.3.4 Solutions of multi-layered pavements ... 101

4.4 Summary ... 104

CHAPTER 5 EFFECT OF MATERIAL CROSS-ANISOTROPY AND HETEROGENITY ON SHAKEDOWN SOLUTIONS OF PAVEMENTS .. 105

5.1 Introduction ... 105

5.2 Effect of material cross-anisotropy ... 106

5.2.1 Problem definition ... 106

5.2.2 Review of the lower bound shakedown approach for a half-space with anisotropic materials (Wang and Yu 2014) ... 111

5.2.3 2D FE model ... 112

5.2.4 3D FE model ... 113

5.2.5 2D solutions and discussions of single-layered problems ... 113

5.2.6 Solutions and discussions of two-layered pavements ... 117

5.3 Effect of material heterogeneity ... 131

5.3.1 Problem definition ... 131

5.3.2 Solutions and discussions of single-layered pavements ... 131

5.3.3 Solutions of two-layered pavements ... 134

viii CHAPTER 6 EXPERIMENTAL STUDY OF SHAKEDOWN CONCEPT

FOR BITUMINOUS PAVEMENTS ... 140

6.1 Introduction ... 140

6.2 The Materials ... 141

6.2.1 Asphalt mixture ... 141

6.2.2 Granular material ... 142

6.3 Determination of Material Characterisatics ... 144

6.3.1 Compaction-related tests on crushed granite ... 144

6.3.2 Monotonic triaxial tests on crushed granite ... 147

6.3.3 Monotonic triaxial tests on asphalt ... 158

6.3.4 Unconfined uniaxial tests on asphalt ... 161

6.4 Wheel Tracking Test ... 168

6.4.1 Wheel tracking facility ... 168

6.4.2 Specimen preparation ... 169

6.4.3 Test procedures ... 172

6.4.4 Determination of contact area and contact pressure ... 173

6.4.5 Experimental results ... 174

6.4.6 Comparisons with theoretical solutions ... 175

ix CHAPTER 7 A COMPARISON BETWEEN THE SHAKEDOWN DESIGN APPROACH AND THE ANALYTICAL DESIGN APPROACH IN THE UK

FOR FLEXIBLE PAVEMENTS ... 179

7.1 Introduction ... 179

7.2 A typical pavement problem ... 180

7.3 Thickness design ... 181

7.4 Influence of temperature ... 183

7.5 Summary ... 189

CHAPTER 8 CONCLUDING REMARKS ... 190

8.1 Conclusions ... 190

x

**LIST OF FIGURES **

Figure 2-1 Typical shakedown behaviours of pavement materials under cyclic

loading ... 8

Figure 2-2 Typical configuration of bituminous pavements (after Thom 2008) ... 12

Figure 2-3 Ideal force distribution through the bituminous pavement (Sharma et al. 2013) ... 12

Figure 2-4 Rutting characteristics ... 13

Figure 2-5 Measurement of the depth and width of the rut on pavement surface (Pedro and Serigos 2012) ... 14

Figure 2-6 Fatigue cracking of pavements ... 14

Figure 2-7 Critical locations in bituminous pavements ... 18

Figure 2-8 Mohr circles and failure envelope... 19

Figure 2-9 Idealised strain response of an asphalt mixture (Gibb 1996) ... 21

Figure 2-10 Accumulation of permanent deformation of asphalt mixture under repeated load (Khanzada 2000) ... 22

Figure 2-11 Vertical permanent strain rate versus vertical permanent strain in log scale (Werkmeister et al. 2004). ... 29

xi Figure 2-12 Schematic of Large-scale model equipment used for prototype

testing at the University of Wisconsin-Madison (Kootstra et al.

2010) ... 30

Figure 2-13 Measured residual stresses in soil after rolling passes (Radovsky and Murashina 1996) ... 31

Figure 2-14 Sydney pavement testing facility ... 32

Figure 2-15 A small wheel tracker at the University of Nottingham (Juspi 2007) ... 33

Figure 2-16 Diagram of the Nottingham Slab Test Facility (Juspi 2007) ... 34

Figure 2-17 Variation of the vertical permanent deformation of Crushed Granite Portaway Sand with number of passes for various wheel pressures (Juspi 2007) ... 34

Figure 2-18 The Nottingham pavement test facility (Juspi 2007) ... 35

Figure 2-19Two-dimensional linear elements ... 42

Figure 2-20 Two-dimensional quadratic elements ... 42

Figure 2-21 A 3D reduced integrated quadratic solid element (C3D20R) ... 42

Figure 3-1 Idealised pavement model and 2D Hertz load distribution ... 44

Figure 3-2 Model sketch and boundary conditions ... 46

Figure 3-3 FE model of plane strain half-space under moving surface load .... 52

Figure 3-4 Residual stresses in Region A upon the removal of load when =
20º, = 20º, *p*0 = 7.56c, single layer model ... 53

Figure 3-5 Residual stress fields after 20 load passes when = 20 º, = 20 º, *p*0
= 7.56c, single layer model ... 53

xii Figure 3-6 Comparison between FE calculated residual stress field and critical

residual stress fields when = 20º, = 20º, *p*0 = 7.56c ... 54

Figure 3-7 Indication of yielding areas in Region A before and after loading passes ... 59

Figure 3-8 Development of plastic normal strain ... 60

Figure 3-9 Development of plastic shear strain ... 61

Figure 3-10 Development of horizontal residual stresses... 62

Figure 3-11 Comparison between critical and numerical residual stress fields in a two-layered pavement ... 64

Figure 3-12 Shakedown limits versus stiffness ratio h1/*a* = 2 and 1 = *ψ*1 = 30°
... 65

Figure 3-13 Numerical shakedown limits in two-layered pavements with varying strength ratio ... 66

Figure 3-14 Layer thickness and materials design of a four-layered pavement 68 Figure 3-15 Mesh distribution in Region A for four-layered pavement model 68 Figure 3-16 Comparison between critical and numerical residual stress fields in a four-layered pavement ... 69

Figure 3-17 3D Hertz pressure distribution ... 70

Figure 3-18 3D model sketch ... 71

Figure 3-19 3D FE model for numerical shakedown analysis ... 74

Figure 3-20 Location of yielding areas in a 3D model ... 75

Figure 3-21 Distributions of the residual stresses after four load passes when *ϕ*
= 0° ... 75

xiii
Figure 3-23 Residual stress fields after four load passes when *p*0 = 4.5c and *ϕ* =

0° when y = 0 ... 77 Figure 3-24 Development of horizontal residual stress xxr under successive

load passes when *ϕ* = 0° ... 78
Figure 3-25 Plastic strain fields at *y* = 0 after four load passes when *p*0 = 4.5c

and *ϕ* = 0° ... 79
Figure 3-26 Residual distortions (deformation scale 600) ... 79
Figure 4-1 Indication of yielding areas in Region A subjected to a static load

following 10 load passes (*p*0 = 10.6c, = 30º) ... 84

Figure 4-2 Development of horizontal residual stress field ... 85
Figure 4-3 Influence of dilation angle on horizontal residual stress field when
= 30º, *p*0 = 10.6c ... 87

Figure 4-4 Influence of dilation angle on horizontal residual stress field when
= 20º, *p*0 = 7.5c ... 88

Figure 4-5 Comparison between FE calculated residual stress field and critical
residual stress fields when = 30º, = 10°, *p*0 = 10.0c ... 89

Figure 4-6 Development of plastic normal strains ... 90 Figure 4-7 Development of plastic shear strains ... 91 Figure 4-8 Comparison of numerical and theoretical shakedown limits for

layered pavements when 1 = 30º, 2 = 0°, c1/c2 = 1 ... 93

Figure 4-9 Influence of plastic flow rule on residual stress field in layered
pavements when 1 = 30º, 1 = 0°, c1/c2 = 1, E1/E2 = 3, *p*0 = 6.7c2

xiv Figure 4-10 Comparison between FE calculated residual stress field and critical

residual stress fields for a layered pavement when 1= 30º, 1=

0°, 2 = 2= 0°, c1/c2 = 1, E1/E2 = 3, *p*0 = 5.5c2 ... 94

Figure 4-11 Comparison of theoretical and numerical shakedown limits for single layered pavements ... 98 Figure 4-12 Dual-wheel Hertz pressure distribution ... 99 Figure 4-13 Comparison of theoretical and numerical shakedown limits with

varying stiffness ratio when 1 = 30°, 2 = *ψ*2 = 0°, c1/c2 = 1 ... 102

Figure 4-14 Comparison of theoretical and numerical shakedown limits in two-layered pavements with varying strength ratio when 1 = 30°, 2

= *ψ*2 = 0°, E1/E2 = 5 ... 102

Figure 4-15 Comparison of theoretical and numerical shakedown limits in two-layered pavements with varying first layer thickness when 1 =

30°, 2 = *ψ*2 = 0°, E1/E2 = 3, c1/c2 = 1 ... 103

Figure 5-1 2D problem definition and Hertz normal and shear stress

distribution (Wang 2011) ... 106 Figure 5-2 3D Problem definition (Wang 2011) ... 109 Figure 5-3 3D FE model ... 113 Figure 5-4 Lower bound shakedown limits versus cv/ch for single-layered

pavements with cross-anisotropic materials ... 115 Figure 5-5 Influence of frictional coefficient on shakedown limits of

single-layered pavements with cross-anisotropic materials when = 0° ... 116

xv Figure 5-6 Design of a two-layered pavement system with cross-anisotropic

materials ... 117 Figure 5-7 Influences of the factor of anisotropy in a 3D sand-clay system .. 122 Figure 5-8 Influences of the factor of anisotropy in a 3D asphalt-clay system

... 123 Figure 5-9 Influence of the factor of anisotropy in a 2D sand-clay system ... 124 Figure 5-10 Influence of the factor of anisotropy in a 2D asphalt-clay system

... 125 Figure 5-11 Influences of plastic cross-anisotropy in a 3D sand-clay system 127 Figure 5-12 Influences of plastic cross-anisotropy in a 3D asphalt-clay system

... 128 Figure 5-13 Definition of heterogeneity problems ... 131 Figure 5-14 Influence of material heterogeneity on 2D shakedown limits of

single-layered pavements ... 133 Figure 5-15 Influence of material heterogeneity on 3D shakedown limits of

single-layered pavements when = 0 ... 134 Figure 5-16 Influence of material heterogeneity in 3D two-layered pavements

when E1/E2 = 1.39, c1/c2 = 20, 1 = 0.4, 2 = 0.3, 1 = 2 = 30 136

Figure 5-17 Influence of material heterogeneity in 2D two-layered pavements when E1/E2 = 1.39, c1/c2 = 20, 1 = 0.4, 2 = 0.3, 1 = 2 = 30 137 Figure 6-1 Current gradation relation of the aggregate in asphalt (refer to BS

EN 12679-5 2009) ... 142 Figure 6-2 Photo of crushed granite (Taken by author 2015) ... 143 Figure 6-3 Particle size distribution of crushed granite sample ... 143

xvi

Figure 6-4 Stress and strain characteristics of sands (Goetz 1989) ... 144

Figure 6-5 Performance of sand under contraction ... 145

Figure 6-6 General set-up of a soil specimen inside a triaxial cell (Rees 2013) ... 149

Figure 6-7 Illustration of triaxial test ... 149

Figure 6-8 GDS triaxial automated system ... 150

Figure 6-9 Preparation of the specimen ... 151

Figure 6-10 Stress and strain responses for dry specimens under different confining pressures ... 153

Figure 6-11 Confining pressures against stiffness moduli for dry specimens 154 Figure 6-12 Mohr circles and the failure line for dry specimens ... 155

Figure 6-13 Stress and strain responses for fully-saturated specimens under different magnitudes of confining pressure ... 157

Figure 6-14 Confining pressures against stiffness moduli for fully-saturated specimens ... 157

Figure 6-15 Mohr circles and the failure line of fully-saturated specimens ... 158

Figure 6-16 Instron apparatus at the University of Nottingham ... 159

Figure 6-17 Photographs of the triaxial chamber for the Instron apparatus at the University of Nottingham (Taken by author 2015) ... 160

Figure 6-18 Mohr circles and the failure line of asphalt mixture ... 161

Figure 6-19 Asphalt specimen set-up for axial compression test ... 164

Figure 6-20 Determination of the stiffness modulus of asphalt during loading or unloading period when ts = 0.05s ... 165

xvii Figure 6-21 Effect of loading and unloading time on stiffness modulus of

asphalt ... 166

Figure 6-22 Stress-strain response of asphalt under dynamic load with a frequency of 2Hz ... 167

Figure 6-23 Effect of loading frequency on stiffness modulus of asphalt ... 168

Figure 6-24 Nottingham wheel tracking facility ... 170

Figure 6-25 Measurement of the wheel load applied on the specimen surface (Taken by author 2015) ... 171

Figure 6-26 Photographic of special designed LVDT (Taken by author 2015) ... 171

Figure 6-27 Bituminous pavement structure ... 172

Figure 6-28 Length of contact patch against contact load ... 173

Figure 6-29 Development of surface deformation under different magnitudes of moving surface load ... 176

Figure 6-30 Change of permanent vertical strain rate against surface deformation ... 178

Figure 7-1 A flexible pavement structure and material properties ... 180

Figure 7-2 Comparison of DBM thickness designs ... 185

Figure 7-3 Comparison of HRA thickness designs ... 185

Figure 7-4 Comparison between analytical design curves and shakedown-based design ... 186

Figure 7-5 Influence on temperature on asphalt stiffness ... 186

Figure 7-6 Pavement shakedown limits for various values of asphalt cohesion and stiffness (kPa) ... 188

xviii Figure 7-7 Influences of asphalt stiffness and layer thickness on the shakedown limit (c1 = 150kPa) ... 188

xix

**LIST OF TABLES **

Table 2-1 Summary of Mohr-Coulomb parameters of asphalt ... 23

Table 3-1 Material parameters for model validation ... 50

Table 3-2 Influence of model dimension ... 50

Table 3-3 Influence of mesh density in the 2D FE model ... 55

Table 3-4 Comparison of numerical shakedown limits for single-layered pavements ... 56

Table 3-5 Comparison of numerical shakedown limits for multi-layered pavements ... 57

Table 3-6 Parameters for the two layered soil material ... 58

Table 3-7 Influence of mesh density on 3D numerical shakedown limits ... 71

Table 4-1 Material parameters and shakedown limits for single-layered pavements ... 83

Table 4-2 Dimensionless lower bound shakedown limit parameters ... 100

Table 4-3 Shakedown limits for single layered-pavement under dual-wheel pressure ... 100

Table 5-1 Comparison of shakedown limits for cross-anisotropic Winnipeg Clay ... 114

xx Table 5-2 Summary of material properties and shakedown limits in

consideration of elastic cross-anisotropy in a 3D sand-clay system ... 120 Table 5-3 Summary of material properties and shakedown limits in

consideration of elastic cross-anisotropy in a 3D asphalt-clay system ... 121 Table 5-4 Summary of material properties and shakedown limits in

consideration of plastic cross-anisotropy in a 2D sand-clay system ... 129 Table 5-5 Summary of material properties and shakedown limits in

consideration of plastic cross-anisotropy in a 2D asphalt-clay system ... 130 Table 5-6 Effect of material heterogeneity on 2D shakedown limits of

single-layered pavements ... 135 Table 5-7 3D shakedown limits for two-layered pavements with heterogeneous materials when E1/E2 = 1.39, 1 = 0.4, 2 = 0.3, 1 = 2 = 30 . 138 Table 5-8 2D shakedown limit for two-layered pavements with heterogeneous

materials when E1/E2 = 1.39, c1/c2 = 20, 1 = 0.4, 2 = 0.3, 1 = 2

= 30 ... 138 Table 6-1 Compaction degree and density index (Djellali at al. 2012) ... 147 Table 6-2 Stiffness moduli and peak axial stresses during shear under different confining pressures for dry specimens ... 154 Table 6-3 Stiffness moduli and axial stresses for fully-saturated specimens

xxi Table 6-4 Maximum axial stress under different confining pressure for asphalt

... 160 Table 6-5 Summary of the stiffness moduli for asphalt specimens tested under

static loads ... 165 Table 6-6 Measurements of the stiffness of asphalt specimens with different

load frequencies ... 167 Table 6-7 transformational relation between the wheel load and the applied

weights on the loading hanger ... 169 Table 6-8 Calculations of the contact length under different magnitudes of load

... 174 Table 6-9 Theoretical shakedown solutions obtained from the present study for comparison with the experimental results ... 177 Table 7-1 Shakedown limit of each layer for a DBM pavement ... 187 Table 7-2 Shakedown limit of each layer for a HRA pavement... 187

xxii

**NOTATION **

*a * half contact width for two-dimensional surface loads and radius of
circular contact area for three-dimensional surface loads

AASHO American Association of State Highway Officials

AASHTO American Association of State Highway and Transportation Officials

c cohesion

ch cohesion on horizontal plane

cn cohesion of nth layer

cv cohesion on vertical plane

c cohesion on a plane inclines at an angle to the horizontal plane

c* modified cohesion considering non-associated plastic flow

plastic strain rate

CBR California Bearing Ratio

CSR Cyclic Stress Ratio

DBM dense bitumen macadam

*P*
*ij*

xxiii HRA hot rolled asphalt

E Young’s modulus (or stiffness modulus)

Eh Young’s modulus in horizontal direction

Em stiffness modulus of asphalt

En Young’s modulus (or stiffness modulus) of nth layer

ET stiffness modulus of asphalt at a specified temperature

Ev Young’s modulus in vertical direction

E0 Young’s modulus at the top surface

E0n Young’s modulus at the top surface of nth layer

FE finite element

*f* yield condition
G shear modulus

Gvh shear modulus in VH plane

*H * height

*hn* thickness of *n*th layer

*ID* density index

*k * dimensionless lower bound shakedown limit

xxiv

*L * length of loading area
length of unloading area

*m*g maximum dry mass

N number of load application to failure

*P * total normal load
normal contact pressure

maximum normal contact pressure

*P*sd actual shakedown limit

*PIr * recovered penetration index

*Q * total shear load

*q * shear contact stress

maximum shear contact stress

*S*T structure surface area where external load are applied

*SPr* softening point
*T*0i external load
*T * temperature
*t * time
*t-1* frequency
'

*L*

*p*0

*p*0

*q*

xxv

𝑢_{𝑖}̇ displacement velocity

*V * volume

*V*m maximum volume reading

VB volume of binder in asphalt

VV volume of air voids in asphalt

VMA voids in mixed aggregate

x, y, z global coordinates x’, y’, z’ local coordinates

*xz* shear strain

t tensile strain at the bottom of the asphalt layer

z normal strain on the top of the subgrade

plastic strain tensor

𝜀_{𝑖𝑗}𝑘̇ _{kinematically admissible plastic strain rate cycle }

accumulated permanent strain after n load cycles

dimensionless load parameter

lower bound shakedown limit parameter

lower bound shakedown limit parameter for *n*th layer

*p*
*ij*

###

*n*

*p*ˆ

*sd*

*n*

*sd*

xxvi

surface frictional coefficient

ij total stress tensor

ije elastic stress tensor

ijr residual stress tensor

1 maximum principle stress/axial stress

3 minimum principle stress/confining pressure

d average density of specimen

max
*d*

###

maximum possible dry densitymin
*d*

###

minimum possible dry density

heterogeneity factor

*n* inhomogeneous ratio of the nth layer

friction angle

friction angle of *n*th layer

* modified friction angle considering non-associate plastic flow

dilation angle

dilation angle of *n*th layer
Poisson’s ratio
*n*
*n*

xxvii Poisson’s ratio regarding the effect of horizontal strain on

complementary horizontal strain

Poisson’s ratio regarding the effect of vertical strain on horizontal strain

Poisson’s ratio of *n*th layer

strain increments
stress increments
2D two-dimensional
3D three-dimensional
*hh*
*vh*
*n*
ij
δε
ij
δσ

1

**CHAPTER 1**

**INTRODUCTION **

**1.1**

**Background **

Shakedown is concerned with the responses of an elastic-plastic structure subjected to cyclic or repeated loads. According to Yu (2006), when the applied cyclic load is above the yield limit but lower than a critical load limit, termed as ‘shakedown limit’, the structure may exhibit some initial plastic deformation; however, after a number of load cycles, the structure ceases to experience any further plastic strain and responds purely elastically to the subsequent load. This phenomenon is called ‘shakedown’. Otherwise, if the load is higher than the shakedown limit, the structure will continue to exhibit plastic strains (known as ratchetting) for however long the load cycles are applied.

Pavement structural design is a process intended to find the most economical combination of layer thicknesses and material types against design traffic. One major distress form considered in the design of bituminous pavements is excessive rutting, which is mainly caused by the accumulation of permanent deformation under repeated traffic loads. Shakedown analysis, based on

elastic-2 plastic theory, can obtain the maximum admissible load (shakedown limit) of a structure against unlimited increasing of permanent deformation under repeated loads; therefore, it is possible to be applied to the structural design of bituminous pavements (Brown et al. 2012).

Actually the shakedown phenomenon has been observed in field tests (Radovsky and Murashina 1996; Sharp and Booker 1984), triaxial tests (e.g. Brown et al. 2008; Larew and Leonard 1962; Lekarp and Dawson 1998; Werkmeister et al. 2001, 2005; Werkmeister 2003; Ravinda and Small 2008) and wheel tracking tests (Brown 2008; Juspi 2007; Kootstra et al. 2010). The range of shakedown limit can be roughly estimated by evaluating the developing tendency of permanent vertical deformation.

Besides, shakedown limits can be determined by using either direct theoretical shakedown analysis or numerical elastic-plastic analysis. In the past few decades, theoretical solutions for shakedown limits of pavements were developed mainly based on two fundamental shakedown theorems (i.e. Melan’s static shakedown theorem and Koiter’s kinematic shakedown theorem). On the one hand, different methods based on Melan’s static shakedown theorem were developed for Tresca or Mohr-Coulomb materials subjected to two-dimensional (2D) and three-dimensional (3D) repeated moving surface loads (e.g. Johnson 1962; Sharp and Booker 1984; Yu and Hossain 1998; Shiau and Yu 2000; Yu 2005; Krabbenhøft et al. 2007; Zhao et al. 2008; Wang 2011; Yu and Wang 2012; Wang and Yu 2013a, 2013b, 2013c, 2014). On the other hand, shakedown analyses using Koiter’s kinematic shakedown theorem have been carried out for 2D and 3D pavement problems (Collins and Cliffe 1987; Collins et al. 1993a, 1993b; Ponter

3 et al. 1985; Collins and Boulbibane 1998; Collins and Boulbibane 2000; Ponter and Engelhardt 2000; Boulbibane et al. 2005; Boulbibane and Ponter 2005a, 2005b; Ponter et al. 2006; Li and Yu 2006). It should be noted that the static and kinematic shakedown solutions provide lower and upper bounds to the true shakedown limit respectively. This is because the static shakedown theorem satisfies the internal equilibrium equations and the stress boundary conditions, while the kinematic shakedown theorem satisfies the compatibility condition for plastic strain rate and boundary conditions for velocity instead. Nevertheless, some identical solutions have been noticed. For instance, when a 2D Mohr-Coulomb half-space is subjected to a repeated moving pressure, the lower bound shakedown solutions (Yu 2005; Yu and Wang 2012) are identical to the upper bound shakedown solutions (Collins and Cliffe 1987). Therefore, upper and lower bound solutions provide exact shakedown limits for those problems. In terms of numerical elastic-plastic analysis, a numerical step-by-step approach was developed by investigating the development of residual stress field in cohesive-frictional half-space under repeated moving surface loads (e.g. Wang 2011; Wang and Yu 2013a).

However, most of the existing solutions are for pavement foundations composed of granular materials and soils. Very limited work has been reported on bituminous pavements. Besides, previous studies usually assume homogeneous, isotropic pavement materials obeying an associated plastic flow rule which is not true in reality.

4

**1.2**

**Aims and objectives **

The research objectives can be concluded as follows:

To give a clear perspective of the shakedown concept and highlight the pivotal role of residual stress field in shakedown analysis.

To obtain shakedown limits of multi-layered pavements and examine the effect of layer configuration on the shakedown limits.

To reveal the influence of non-associated plastic flow rule of materials on the shakedown limits of pavements.

To study the effect of anisotropy and heterogeneity of materials on the shakedown limits by further developing a lower bound shakedown approach.

To validate the shakedown concept in layered bituminous pavements by wheel tracking tests.

To directly compare the shakedown-based pavement design approach and the analytical design approach adopted in the UK Design Manual for Roads and Bridges HD26/06 (Highways Agency 2006).

**1.3**

**Thesis outline **

This thesis is divided into eight chapters. A brief outline is given below:

Chapter 1 provides necessary background information and key objectives of the present study.

5 Chapter 2 gives literature reviews including the notion of shakedown, key aspects of bituminous pavements (typical structure of bituminous pavements, principle distress modes, properties of pavement materials), fundamental shakedown theorems and previous research on pavement shakedown.

Chapter 3 presents a step-by-step approach using 2D and 3D finite element analysis in order to obtain numerical shakedown limits and investigate the development of residual stresses and plastic strains. The effect of layer configuration is also assessed.

Chapter 4 develops both numerical and theoretical shakedown solutions for pavements with materials following a non-associated plastic flow rule. These solutions are compared with numerical shakedown solutions.

Chapter 5 extends the theoretical shakedown approach to pavements with cross-anisotropic or heterogeneous materials.

Chapter 6 presents an experimental work showing responses of a bituminous pavement structure under moving loads. Triaxial and uniaxial compression tests were also conducted to obtain the stiffness and strength parameters which were used to calculate the theoretical shakedown limit, then compared with the experimental shakedown limit.

Chapter 7 applies the lower bound shakedown approach to design layer thicknesses of a typical bituminous pavement and then compares with the existing analytical design approach in the UK.

6 Chapter 8 summarises the major findings in the present study and gives suggestions on future research.

7

**CHAPTER 2**

**LITERATURE REVIEW **

**2.1**

**Introduction **

In this chapter, the basic shakedown concept and two fundamental shakedown theorems are first presented, followed by an introduction to bituminous pavements. Then experimental observations of the shakedown phenomenon and recent shakedown studies in the field of pavement engineering are summarised. Finally, the commercial finite element software ABAQUS is briefly introduced.

**2.2**

**Notion of shakedown in pavements **

Three distinct behaviours, known as purely elastic, shakedown, and incremental collapse respectively, can be recognised when a pavement structure is subjected to different levels of repeated load (Figure 2-1).

Purely elastic behaviour will occur only when the load level is sufficiently small so that no permanent deformation can be observed after unloading.

8 When the applied load is above the yield limit, but lower than a critical load; the structure may deform plastically in initial load cycles, but respond purely elastically to subsequent load cycles. This phenomenon is called ‘shakedown’, and the critical load is termed as the ‘shakedown limit’.

Figure 2-1 Typical shakedown behaviours of pavement materials under cyclic

loading

In terms of the incremental collapse, also known as ratchetting, this is caused by the increase of plastic strain after each cycle of load when the applied load level is relatively high. Ratchetting can result in excessive rutting and thus should be avoided.

**2.3**

**Shakedown theorems **

In the past few decades, shakedown analyses were generally carried out based on two fundamental shakedown theorems, known as Koiter’s kinematic (upper bound) shakedown theorem and Melan’s static (lower bound) shakedown theorem respectively. The advantage of using the shakedown theorems is that detailed stress and strain history are not required during calculation.

Collapse Elastic limit

Shakedown limit

(a) Elastic (b) Shakedown (c) Collapse

9

**2.3.1** **Melan’s static shakedown theorem **

Melan’s static shakedown theorem (Melan 1938) states that an elastic-perfectly plastic structure under cyclic or variable loads will shakedown if a time-independent residual stress field exists such that its superposition with a load-induced elastic stress field does not exceed the yield criterion anywhere in the structure.

(2.1)

where ije is the elastic stress field due to applied unit pressure , is a scale

parameter, ijr is the self-equilibrated residual stress field and *f*(ij) = 0 is the

material yield criterion.

By searching all possible self-equilibrated residual stress fields under pressure , the largest value of (defined as ) can be obtained to ensure the stresses in the structure satisfy Equation (2.1). Thus, is termed as the ‘shakedown limit parameter’ and accordingly, is the actual shakedown limit.

**2.3.2** **Koiter’s kinematic shakedown theorem **

Koiter’s kinematic shakedown theorem (Koiter 1960) states that shakedown cannot occur for an elastic-perfectly plastic structure subjected to cyclic or variable loads if the rate of plastic dissipation power is less than the work rate of external forces for any admissible plastic strain rate cycle. It can be expressed as

(2.2)
0
)
σ
σ
(*λ* e_{ij} _{ij}r
*f*
0u
*p*
0
*p*
_{sd}*sd*
0
*p*
*P _{sd}*

*, ε σ 0 k ij k ij 0 0*

_{sd}###

###

*t*

*V*

*T*

*t*

*S*

*k*

*i*

*iu*

*dS*

*dt*

*dV*

*p*

*dt*

*T*

10 where

is displacement velocity,

*p*0i is external load,

*ST* is the structure surface area where external load is applied,
ij is stress on the yield surface,

*V* is structure volume,

is any kinematically admissible plastic strain rate cycle.

Therefore, it can be known that the structure may shakedown if the inequality sign in Equation (2.2) is reversed:

(2.3)
which provides an upper bound to shakedown load multiplier *λ*sd and therefore

the upper shakedown limit is *λp0*.

**2.4**

**Bituminous pavements **

**2.4.1** **Typical structure of bituminous pavements **

A typical structure for a bituminous pavement is given in Figure 2-2. The surface course, also known as wearing course, is comprised of asphalt (e.g. Hot Rolled Asphalt (HRA), Dense Bitumen Macadam (DBM), Stone Mastic Asphalt (SMA) and so on), so that it can withstand direct loading. Due to the high expenditure,

*i*
*u*
*k*
*ij*

###

*t*

###

###

*t*

*V*

*S*

*k*

*i*

*iu*

*dS*

*dt*

*dV*

*p*

*dt*

*T*0 0 k ij k ij 0 σ ε ,

11 the typical thickness of this layer is relatively thin, varying from 20mm to 50mm. The base layer provides the pavement most of its strength and distributes the imposed wheel load to the pavement foundation; therefore it must be with sufficient quality and sufficient thickness. The thickness of this layer is typically 200mm or more. Generally, larger particle sizes tend to be used, whether the layer is of asphalt (e.g. HRA or DBM) or granular materials. The use of larger particles makes the surface of this layer uneven and therefore the direct application of the wearing course layer may reduce the quality of the finished road surface. Insertion of a binder course layer, made of asphalt with particle size larger than those in course layer, but smaller than those in the base layer, acts a transition between the wearing course layer and the base layer, of which the thickness ranges from 50mm to 80mm typically. The subbase layer is beneath the base layer and serves as the foundation for the overall pavement structure, transmitting traffic loads to the subgrade and providing drainage and frost protection. A typical thickness of 150mm is recommended. Capping layer, a subgrade-improvement layer, is always made of cheap and locally available materials and constructed for poor subgrade only. Generally, crushed gravels and rockfill may be the suitable options of capping materials. Overall, the goal of the bituminous pavement is to distribute the traffic loads down to the subgrade over a sufficiently large area as shown in Figure 2-3 to minimise the stress level on the top of the subgrade (Sharma et al. 2013).

12 Figure 2-2 Typical configuration of bituminous pavements (after Thom 2008)

Figure 2-3 Ideal force distribution through the bituminous pavement (Sharma et al. 2013)

**2.4.2** **Failure modes of bituminous pavements **

Two principal failure modes are of most concern in the design of bituminous pavements: excessive rutting and fatigue cracking.

Rutting is recognised as a permanent downward deformation on the pavement surface induced by repeated wheel loads, which may badly affect comfort, ride

Surface course -asphalt

Sub-base – granular materials Capping (lower sub-base) granular materials (used over poor subgrade; often in more than

one layer)

Subgrade (substrate) - soil Base – granular materials (often in more than one layer)

20-50mm

200mm 50-80mm

200mm Binder course -asphalt

13 quality, motorist safety and some other general performance characteristics of pavements (Haas et al. 1994). Excessive rutting can eventually occur if irrecoverable deformation of pavements keeps rising with increasing number of load passes (Witezak et al. 1997; Fwa et al. 2004). In the UK, the limiting rut depth is often taken to be 25 mm and pavements with rut depth varying from 15 to 20 mm should be considered for remedial work, such as the provision of an overlay or replacement of the surfacing (Croney and Croney 1991). In other countries, the limiting rut depth varies from 15mm to 25mm (De Pont et al. 1999; Jameson and Sharp 2004; Maji and Das 2005).

Measurements of ruts are usually conducted by placing a straight edge across the wheel path as shown in Figures 2-4 and 2-5. Generally speaking, the rut depth reflects the degree of rutting, and the rut width can be used as a sign of which layer has failed; normally a very narrow rut corresponds to a surface failure, while a wide one is indicative of a subgrade failure (Adlinge and Gupta 2013).

14 Figure 2-5 Measurement of the depth and width of the rut on pavement surface

(Pedro and Serigos 2012)

Fatigue cracking occurs due to repeated wheel loading, and perhaps assisted by climatic factors such as low-temperature stress (Thom 2008). The generation of cracks may reduce the ride quality and provide pathways for water to flow into the pavement foundation. Fatigue cracks may start at the bottom of the bituminous layer which is usually considered to be the most critical place where the highest tension stress is expected to occur in the analytical pavement approach in the UK. Then the cracks may propagate to the pavement surface or connect with adjacent cracks (Figure 2-6) and eventually leading to failure of pavements. As the wheel loading continues, more cracks are formed.

15

**2.4.3** **Current pavement design methods **

Nowadays, pavement structural design can be conducted using an empirical approach or a mechanistic-empirical approach. Normally, the empirical approach is achieved by charts and equations developed from experimental and field work. In the aspect of the mechanistic-empirical approach, the concepts of mechanics are utilised together with the empirical equations to predict the performance of pavement structures. In this subsection, some representative methods are reviewed.

The CBR (California Bearing Ratio) method is one of the earliest empirical pavement design approaches developed by California Division of Highways in around 1930 as a result of surveys made during 1928 to 1929 (Yoder and Witczak 1975). CBR is expressed as a percentage of the penetration resistance to that of a standard value for crushed stone. The CBR value can be regarded as a sign of the quality of pavement materials. Some thickness design charts were developed based on the empirical relations established between the CBR value and the thickness. In 1944, this method was adopted by the U.S. Corps of Engineers for the design of airfield pavements (Porter 1950, Corps of Engineers 1945). Following that, the CBR approach was applied in highway design (e.g. Brown and Ahlvin 1961; Highways Agency 2009). Hveem and Carmany (1949) modified the traditional CBR design approach by further considering the cohesion and friction of granular materials.

The empirical design approach recommended by the American Association of State Highway Transportation Officials (AASHTO) was developed based on the

16 test results of the American Association of State Highway Officials (AASHO) road in-situ tests conducted in Ottawa, Illinois from 1956 to 1958. These in-situ tests involved observations of the performance of pavements at the end of selected time periods. Some physical features of the pavements, including longitudinal roughness, rutting depth in wheel tracks and extent of cracking and patching, were assessed (AASHTO 1972). The AASHO design equations were developed based upon a statistical analysis of the test data. Even though the AASHO tests provide a significant contribution to pavement design, their limitations are obvious. The design formula is applicable to specific pavement structures under a specific environment only. Again, it is difficult to predict the twenty-year performance of a pavement from a two-year test.

The mechanistic-empirical design is achieved by first obtaining elastic data (e.g. stress, strain, deflection) of a pavement structure under design loads, then inputting these data into selected empirical models to predict pavement responses (e.g. rutting, fatigue cracking, low-temperature cracking or smoothness) over the pavement design life. By using this approach, the designer should first select a ‘trial pavement’ with a specified layer configuration and material properties (from laboratory or field tests); then the critical stress and/or strain of the trial pavement due to the design traffic load are analysed to predict the critical life of the pavement based on the empirical models.

The rise of the mechanistic-empirical approach in pavement design can be traced back to 1962, in which year an international conference on the structural design of pavements attracted great attention and laid the foundation for the development of the mechanistic-empirical design approach. Until now, plenty of

17 work has been reported regarding the mechanistic-empirical approach (e.g. Jones 1962; Peutz 1968; Finn et al. 1977; Powell et al. 1984; Brown et al. 1985; Seeds 2000; Nunn 2004). For example, according to the Design Manual for Roads and Bridges HD26/06 (Highways Agency 2009), TRRL Report LR1132 provides guidance that should be considered in the preparation of mechanistic-empirical design for bituminous pavements, also known as analytical design approach in the UK. Two principal failure modes are considered in this approach: fatigue cracking and excessive rutting. While the excessive horizontal tensile strain at the bottom of the bound layer r leads to fatigue cracking, the excessive

vertical compressive strain at the top of subgrade z is related to pavement rutting

(Figure 2-7). Empirical equations are used to link the pavement life with the critical strains. Report LR1132 suggested the following empirical correlations for Dense Bitumen Macadam (DBM) and Hot Rolled Asphalt (HRA) at 20°C:

Criterion against fatigue:

, for DBM (100pen) (2.4)

, for HRA (50pen) (2.5)

Criterion against rutting:

z 3.95logε -7.21 -N log , (2.6)

where Nis the number of standard axles (in millions).

r ε log 16 . 4 38 . 9 N log r ε log 32 . 4 78 . 9 N log

18 .

Figure 2-7 Critical locations in bituminous pavements

**2.5**

**Properties of pavement materials **

**2.5.1** **Granular materials **

Properties of granular materials can be described in two aspects: stiffness and strength. Stiffness is the ratio of the applied stress to the induced strain. Stiffness of granular material is not like that of linear elastic materials; it may vary depending on the stress condition. In the aspect of strength, friction angle and cohesion are two main factors used to describe the shear strength of granular materials.

Both the stiffness and the strength of granular materials can be measured by the triaxial test. Since the granular material does not behave purely elastically under

a pressure, a secant modulus is recommended to be used as the stiffness modulus of granular material. This is done by taking the slope of a secant between two points on the stress-strain curve (Poulos and Davis 1980; Briaud 2001; Ranjan

Horizontal tensile strain Asphaltic layer

Base and sub-base layer

Subgrade

19

and Rao 2007). Lambe and Whitman (2008) stated that normally the stiffness modulus is the secant modulus from zero to a deviator stress (1-3) equal to

one-third to one-half of the peak deviator stress. Besides, Briaud (2001) proposed that the stiffness modulus can be calculated by:

, (2.7)

in which E is the stiffness modulus, 1 is the axial stress, 3 is the confining

pressure, zz is the vertical strain and is the Poisson’s ratio. If a maximum

Poisson’s ratio (0.5) is selected, the secant modulus agrees with that in Lambe and Whitman (2008).

c and *ϕ*can be determined by seeking a well-matching failure line for couples of
Mohr circles plotted by using the triaxial test data (Figure 2-8). By simplifying
the Mohr-Coulomb envelope as a straight line, the Mohr-Coulomb yield
criterion can be written in a linear form relating to c and *ϕ*.It is considered that
any stress state exceeds this line is considered to be yield.

Figure 2-8 Mohr circles and failure envelope
zz
3
1
ε
σ
2
σ
E *ν*

20 However, stiffness modulus measured by means of triaxial test under repeated loads (Elliot and Thornton 1988; Puppala et al. 1996; CEN 2004; AASHTO 2007) is more realistic for pavement design. It was found that the stiffness modulus increase slightly after each load cycle, but to a first approximation it can be considered to be constent (Thom 2008). Therefore, in a relatively loose sense, stiffness modulus obtained from monostatic triaixial test is reasonable to be used in pavement design.

**2.5.2** **Asphalt **

Asphalt is basically a granular material with an added binding ingredient (i.e. bitumen). The addition of bitumen affects the property of asphalt undeniably. Therefore, it is necessary to know the properties of bitumen and how do they affect the properties of asphalt. Bitumen behaves as an elastic solid under quick loading or at low temperatures, while acts as a viscous fluid at high temperature or under slow loading. Due to the addition of bitumen, deformation of asphalt should be concerned with the elasticity, visco-elasticity, viscosity and plasticity (Figure 2-9).

The uniaxial compression test has been employed in determining the stiffness modulus of asphalt. Deng (2000) indicated that asphalt performs purely elastically at a low temperature or under a very quick loading (last around 10-8 s to 10-6 s). However, most tests are conducted at a considerably slow errate due to the limitation of test equipment. Stiffness modulus actually involves the combined effects of elasticity and visco-elasticity. More details about the uniaxial compression test will be mentioned in Section 6.3.4.

21 Deformation of asphalt consists of two parts: recoverable deformation and permanent deformation (Figure 2-9). The recoverable part can be instantaneously recovered or gradually recovered. The gradually recovered deformation is due to visco-elasticity of asphalt.

Thom (2008) indicated that the magnitude of strain taking place within the aggregate skeleton is relatively small compared with those encountered in unbound materials as the binder takes much of the stress away from the particle contacts. With an increase of temperature, the stresses across particle contacts increase and result in an increaseed danger of inter-particle slips (from particle rotation and separation). Accumulation of the permanent deformation in asphalt is illustrated in Figure 2-10.

22 Figure 2-10 Accumulation of permanent deformation of asphalt mixture under

repeated load (Khanzada 2000)

The Mohr-Coulomb yield criterion has also been suggested to describe the strength of asphalt (e.g. McLeod and Ricketts 1950; Endersby 1951; Goetz 1989, Smith 1951; McLeod 1952; Road Research Laboratory 1962; Fwa et al. 2001, 2004; Witzcak 2002; Airey and Prathapa 2013). Hence, the plastic properties of asphalt can be described by friction angle () and cohesion (c) at a specified temperature. Table 2-1 summarises the strength data for standard hot mix asphalt (HMA). Some experimental results of the friction angle and cohesion of hot rolled asphalt at 30°C from triaxial tests were given were given in the report of Road Research Laboratory (1962). The results demonstrate that the change of the aggregate type from sand to stone may increase the cohesion of asphalt to some extent, while decreasing the friction angle. Moreover, the decrease of binder content may increase the cohesion; however its effect on the friction angle is minor. Furthermore, Chen et al. (2009) reported that there exist two optimum binder contents which can provide the maximum cohesion and the maximum frictional angle respectively. They also noted that increasing binder viscosity

23 may lead to higher values of cohesion and friction angle. Fwa et al. (2004) carried out triaxial tests on three types of asphalt at different temperatures. The results show that higher temperature may reduce the cohesion but increase the friction angle. However, Chen at al. (2009) reported that the increasing temperature may lead to smaller cohesion as well as smaller friction angle. In summary, the effect of temperature on the friction angle is uncertain. Nevertheless, it can be found from both Fwa et al. (2004) and Chen et al (2009) that the change of temperature does not influence the friction angle very much. This agrees with Goetz’s (1989) statements which indicate that the friction angle is affected minimally by test temperature. In summary, the strength properties of the asphalt mixture depend on various factors. For example, aggregate grading obviously affects the friction angle, while the binder (bitumen) content and grade influence the material cohesion. This may explain the wide range of values in Table 2-1.

Table 2-1 Summary of Mohr-Coulomb parameters of asphalt

Reference Type of asphalt

mixture T (°C) c (kPa) (°) Airey and Prathapa (2013) SMA NA NA 34.6

DBM NA NA 41

Bindu and Beena (2013) SMA 60 109 35

Chen et al. (2009) SMA 25 420 43.3 40 245 42.8 60 204.4 38.6 Christensen et al. (2002) NA 20 571-933 20.4-44.8 Fwa et al. (2004) NA 28 1768.8 15.1 40 616.4 33.4 60 290.0 36 Zofka et al. (2014) NA 25 760-1110 13.8-57.5

24

**2.5.3** **Associated and non-associated plastic flow rule **

Determining the amount of plastic strain relates to a concept in plasticity known as plastic flow. It is well known that the failure surface defines the boundary of elastic deformation. When the stress state reaches the failure surface, further loading induces plastic flow. For an elastic-perfectly-plastic model, the stress state satisfying the yield condition will become unchanged, but will cause unlimited plastic strain. Clearly, there is no straightforward relationship between the yield stress and the plastic strain. Therefore, a strain rate is introduced which is defined as the rate at which the strain increases with respect to time.

Two rules were established to define the relation between the components of plastic stresses and the corresponding plastic strain rates, named as associated plastic flow rule and non-associated plastic flow rule.

An associated plastic flow rule has been confirmed by many experiments on
frictionless materials (e.g. metals), of which the vector of plastic strain rate is
normal to the yield surface. Therefore, the plastic strain rate ( ) can be
described as a function relating to the yield criterion (*f*):

(2.8)

in which the scalar *dλ* represents a proportional coefficient that can change with
loading.

However, the associated plastic flow has not been successfully implemented for cohesive-frictional materials (e.g. soil and rocks), as its application in granular materials may overestimate the volume changes during plastic failure (Scott

*p*
*ij*
*d*
*ij*
*p*
*ij*
*f*
*d*
*d*

25 2013). Non-associated plastic flow is therefore proposed by assuming that the plastic strain rate is not normal to the yield surface, but to a plastic potential surface of which the function is in a form very similar to the yield function as shown in Equation (2.9) (Nova and Wood 1978; Lade et al. 1987, 1988).

(2.9)

For Mohr-Coulomb materials, the plastic potential surface is defined by replacing the friction angle () with a dilation angle (). In other words, if an associated plastic flow rule is applied, the dilation angle () is equal to the friction angle (); otherwise, the dilation angle is smaller than the friction angle and may be close to 0.

**2.5.4** **Material anisotropy **

The materials which are assumed to have a single vertical axis of symmetry with the same properties in any horizontal direction, but different properties in the vertical direction are known as cross-anisotropic or transverse isotropic materials. According to Wang and Yu (2014), Ev/Eh and cv/ch can be regarded as

the two main indexes to evaluate the elastic anisotropy and plastic anisotropy of materials, in which E is Young’s modulus and c is cohesion, h and v relate to the horizontal plane and vertical plane respectively.

Elastic properties of anisotropic soils have been widely explored. For example, typical values of Ev/Eh for clays may range from 0.25 to 1.11 (e.g. Yu and

Dakoulas 1993; Lings et al. 2000; Yimsir and Soga 2011). Experimental results for sands and gravel also show some degree of inherent anisotropy with Ev/Eh

*ij*
*p*
*ij*
*Q*
*d*
*d*

26 from 1.06 to 2 (e.g. Hoque et al. 1996; Jiang et al. 1997; Kuwano and Jardine 2002). The property of anisotropy is also an inherent characteristic of asphalt concrete caused by the non-uniform distribution of aggregates. Experimental data (Wang et al. 2005) show that the anisotropy of asphalt concrete under field compaction might also be approximated as cross-anisotropy with Ev/Eh ≈ 3.33.

Laboratory tests performed on soil specimens cut at different orientations have also demonstrated the directional dependence of soil shear strength (e.g. Lo 1965; Arthur and Menzies 1972; Guo 2008). It has been suggested that the variation of soil cohesion with direction due to inherent anisotropy is much more significant than the anisotropy of friction angles (Arthur and Menzies 1972). The value of cv/ch may relate to the value of Ev/Eh. For example, when the soil is heavily

compressed, Ev/Eh > 1and cv/ch > 1 (Jiang G L et al. 1997). Chen (2013) indicated

that the value of cv/ch is within 0.75 to 2 for clay.

**2.5.5** **Material heterogeneity **

As a layered structure, material properties of these layers are diverse. Even within a single type of material, the material property may also vary at different locations. Typically, the stiffness of soil increases with depth. Some relations have been suggested to describe the change of stiffness modulus with depth. For example, Gibson (1967) assumed that the stiffness modulus changes linearly with depth:

27 in which Ez is the Young’s modulus at depth ‘z’ and k is a constant). This kind

of soil is known as Gibson-type soil. This Gibson soil has been widely applied to solve footing problems (Boswell and Scott 1975; Stark and Booker 1997). Apart from that, some researchers also assumed a power law relation: Ez = E0zk

(where 0 ≤ *k* < 1 is a non-dimensional exponent) (Carrier and Christian 1973)
or an exponential law relation: Ez = E0ez (E0 0 and can be either positive or

negative) (Rowe and Booker 1981; Giannakopoulos and Suresh 1997).

**2.6**

**Previous studies of shakedown in pavement **

**engineering **

**2.6.1** **Experimental observation of shakedown behaviour **

At the beginning, the shakedown phenomenon was observed from triaxial tests. Larew and Leonard (1962) did some undrained repeated triaxial tests on partly-saturated (around 80% saturation degree) granular materials. Results were reported by plotting the permanent deformation against the number of load cycles. A shakedown limit of around 84% to 91% of the maximum compression stress (critical limit 1max) was presented for silty clay. Undrained triaxial tests

were also conducted by Sangrey et al. (1969) and Lashine (1971) on consolidated saturated clay and consolidated Keuper Marl respectively. The obtained shakedown limits ranged from 67% to 85% of 1max.

Tang et al. (2015) conducted undrained tests on fully-saturated clay with selected confining pressure varies from 56 kPa to 85 kPa. The specimens were collected

28 from different depths of the test field. The shakedown or non-shakedown behaviours are classified by introducing a cyclic stress ratio (CSR) which is defined as the ratio between the cyclic shear stress and the consolidated undrained shear strength obtained through monotonic triaxial tests. The results were analysed by plotting the number of load cycles against pore pressure or axial strain. Results demonstrated that the shakedown limits of the clay collected at any depth were all at around CSR = 0.03 and the critical cyclic ratio was at around CSR = 0.44.

Lekarp and Dawson (1998) conducted repeated load triaxial tests on five
different aggregates under drained condition to examine the relations between
the development of permanent axial strain and the number of load applications.
Results indicated that at low levels of shear stress (defined as *q*max/(*p*max+*p**), in

which *q*max is the maximum deviator stress, *p*max is the maximum mean normal

stress and *p** is defined by the intersection of the static failure line and the *p*-axis
in *p/q* space), the growth of permanent strain eventually levels off and reaches
an equilibrium condition, whereas large load level may cause gradual failure.
The equilibrium condition is similar to the shakedown phenomenon. They also
indicated that the model proposed by Paute et al. (1996) can successfully predict
the relations between the permanent axial strain and the number of load
applications under shakedown condition.

Drained triaxial tests were also conducted on diverse granular materials by Werkmeister et al. (2001, 2004, 2005) and Werkmeister (2003) under different magnitudes of loads. Three behaviours were observed as shown in Figure 2-11,

2
/
)
(_{1} _{3}
*cu*

29 in which three different phenomena were defined: plastic shakedown (labelled as A), plastic creep (labelled as B) and incremental collapse (labelled as C). Again, they defined the boundaries for those three ranges as follows, and they have been included in European Standard EN-13286-7.

A: (ˆ5000* _{p}* ˆ

*3000)0.045103, (2.11) B: 3 5000 3000 3 10 4 . 0 ) ˆ ˆ ( 10 045 . 0 *

_{p}*p*

*p* , (2.12) C:(ˆ

*5000ˆ3000*

_{p}*)0.4103, (2.13) in which,*

_{p}_{ˆ}3000

*p* and

_{ˆ}5000

*p*

are accumulated permanent strains after 3000 and 5000 load cycles.

Figure 2-11 Vertical permanent strain rate versus vertical permanent strain in log scale (Werkmeister et al. 2004).

Apart from the repeated triaxial tests, Kootstra et al. (2010) conducted large-scale tests on two-layered specimens by applying repeated cyclic loads (700kPa) (Figure 2-12). The shakedown phenomenon was observed in the base layer of some particular cases.

30
Considering the moving nature of traffic loads, Radovsky and Murashina (1996)
performed a full-scale test to validate the shakedown concept in soil under a
rolling strip of 310kPa. Pressure cells were installed beneath the subgrade
surface at different depths to measure the horizontal residual stresses. The
subgrade soil contained 10% sand, 77% silt and 13% clay and the moisture
content was 15%. Results indicated that the horizontal residual stresses increased
with the number of repeated loads and became constant eventually after 12
rolling passes. The measured residual stresses are plotted in Figure 2-13 which
indicates that the most critical residual stress was beneath the surface at a depth
of around z = 7cm (z/*a* = 0.52, where a is half of the tyre contact length). The
most critical depth is consistent with Wang and Yu (2013a)’s numerical
solutions.

Figure 2-12 Schematic of Large-scale model equipment used for prototype testing at the University of Wisconsin-Madison (Kootstra et al. 2010)

31 (a) Location of pressure cell

(b) Measured residual stresses with depth

Figure 2-13 Measured residual stresses in soil after rolling passes (Radovsky and Murashina 1996)

Ravinda and Small (2008) utilised the Sydney pavement testing facility (Figure 2-14) to investigate the shakedown phenomenon of three kinds of unbound pavement configuration sealed with bitumen emulsion under moving wheel load. Results showed that wheel load lower than the shakedown limit for a large

32 number of load passes results in less deformation than that under a lower number of load cycles of a load larger than the shakedown limit.

Figure 2-14 Sydney pavement testing facility

Brown et al. (2008) carried out tests on four types of soil and granular materials by using a small wheel tracking apparatus or a slab test facility at the University of Nottingham (Figure 2-15 and Figure 2-16). For soil like silty-clay, of which the particle size is relatively small, the small wheel tracking apparatus was employed. All the specimens were contained in a mould of 400mm in length, 280mm in width and 125mm in depth. Wheel loadings were applied by a 200mm diameter steel wheel with a solid rubber tyre of 50mm width. In terms of the slab test facility, it was utilized to test specimens like crushed rock of which the particle size is relatively large. Certainly, a larger specimen needed to be prepared which is 1m long × 0.6m wide × 0.18m deep. The results also revealed three types of phenomenon as shown in Figure 2-17, in which Type 1 is known as shakedown, Type 3 is definitely much in excess of shakedown and the intermediate case is defined as Type 2. The obtained experimental shakedown limit is compared with theoretical predictions and the results show that the